# Polymer Chemistry. The Basic Concepts - Himenz P.C.

**Download**(direct link)

**:**

**139**> 140 141 142 143 144 145 .. 312 >> Next

BB monomers and that the Â groups are present in excess. We define vA and

vB to be the numbers of A and Â functional groups, respectively. The

number of either of these quantities in the initial reaction mixture is

indicated by a superscript 0; the numbers at various stages of reaction

have no superscript. The stoichiometric imbalance is defined by the ratio

r, where

This ratio cannot exceed unity by definition of the problem.

As with other problems with stoichiometry, it is the less abundant

reactant that limits the product. Accordingly, we define the extent of

reaction p to be the fraction of A groups that have reacted at any point.

Since A and Â groups

310

Condensation or Step-Growth Polymerization

react in a 1:1 proportion, the number of Â groups that have reacted when

the extent of reaction has reached p equals pj\°, which, in turn, equals

ðã^â°. The product pr gives the fraction of Â groups that have reacted at

any point. With these definitions in mind, the following relationships

are readily seen:

1. The number of unreacted functional groups after the reaction reaches

extent p is

"a = (1 - P)"a0

(5.35)

and

"â = 0 " Ðã)"â° = 0 " Pr)

(5-36)

2. The total number of chain ends is the sum of Eqs. (5.35) and (5.36):

"end, = (l-P + V-- j^A0

(5-37)

3. The total number of*chains is half the number of chain ends:

Nchai"s = \ (l+^ - 2ð)"à°

(5-38)

4. The total number of repeat units distributed among these chains is

the number of monomer molecules present initially:

Nrepeat units = j ''a + j V = j I1 + " I

(5 39)

(' + rH°

The number average degree of polymerization is given by dividing the

number of repeat units by the number of chains, or

- _ l + l/r _ l+r

, m

Ïï 1 + 1/r- 2p~ l + r - 2pr

^ ^

As a check that we have done this correctly, note that Eq. (5.40)

reduces to the previously established Eq. (5.28) when r = 1.00.

One distinction that should be pointed out involves the comparison

of Eqs. (5.1) and (5.40). In the former we considered explicitly the AB

monomer, while the latter is based on the polymerization of AA and BB

monomers. In both instances nn is obtained by dividing the total number

of monomer molecules initially present by the total number of chains

after the reaction has occurred to extent p. Following the same procedure

for different reaction

Stoichiometric Imbalance

311

mixtures results in a different definition of the repeat unit. In the

case of the AB monomer, the repeat unit is the ab entity, which differs

from AB by the elimination of the by-product molecule. In the case of the

AA and BB monomers, the repeat unit in the polymer is the aabb unit,

which differs from AA + BB by two by-product molecules. Equation (5.1)

counts the number of ab units in the polymer directly. Equation (5.40)

counts the number of aa plus bb units. The number of aa plus bb units is

twice the number of aabb units. Rather than attempting to formalize this

distinction by introducing more complex notation, we simply point out

that application of the formulas of this chapter to specific systems must

be accompanied by a reflection on the precise meaning of the calculated

quantity for the system under consideration. There is nothing

particularly unique about this admonition: No equation should be used

mindlessly by just plugging in numbers and submitting an answer.

The distinction pointed out in the last paragraph carries over to the

evaluation of Mn from nn. We assume that the chain length of the polymer

is great enough to make unnecessary any correction for the uniqueness of

chain ends. In such a case the molecular weight of the polymer is

obtained from the degree of polymerization by multiplying the latter by

the molecular weight of the repeat unit. The following examples

illustrate the distinction under consideration:

1. Polymerization of an AB monomer is illustrated by the polyester

formed from glycolic acid. The repeat unit in this polymer has the

structure

Î

II

(-0-CH2-C-) and M0 = 58. Neglecting end groups, we have Mn = 58 nn,

with nn given by Eq. (5.1).

2. Polymerization of AA and BB monomers is illustrated by butane-1,4-

diol and adipic acid. The aabb repeat unit in the polymer has an M0 value

of 200. If Eq. (5.4) is used to evaluate nn, it gives the number of aa

plus bb units; therefore Mn = 200(nn)/2.

3. An equivalent way of looking at the conclusion of item (2) is to

recall that Eq. (5.40) gives the (number average) number of monomers of

**139**> 140 141 142 143 144 145 .. 312 >> Next